coal for metallurgical coke production: predictions of...
Embed Size (px)
Coal for metallurgical coke production: predictions of coke quality
and future requirements for cokemaking
M.A. Dıez*, R. Alvarez, C. Barriocanal
Instituto Nacional del Carbon (INCAR), CSIC, Apartado 73, 33080 Oviedo, Spain
Accepted 31 October 2001
This paper reviews quality requirements of metallurgical coke for the blast furnace, coke structure, and relationships
between structure and quality. Models of prediction of metallurgical coke quality parameters based on maceral composition and
properties of coals being carbonized are summarized. Early prediction models of cold coke strength and the development of
second-generation hot-strength prediction models based on parameters as coke reactivity index (CRI) and coke strength after
reaction with carbon dioxide (CSR) are assessed. The review concludes with an assessment of current coke production and coal
demand in the steelmaking industry, globally, followed by a preview of possible future alternative coking technologies.
D 2002 Elsevier Science B.V. All rights reserved.
Keywords: Coking coal; Cokemaking; Coke quality; Prediction; Strength; Reactivity; New cokemaking technology
1. Coke for the blast furnace
Metallurgical coke is a macroporous carbon mate-
rial of high strength produced by carbonization of
coals of specific rank or of coal blends at temperatures
up to 1400 K. About 90% of the coke produced from
blends of coking coals is used to maintain the process
of iron production in the blast furnace where it has
three major roles:
1. as a fuel, it provides heat for the endothermic
requirements of chemical reactions and the melting
of slag and metal;
2. as a chemical reducing agent, it produces gases for
the reduction of iron oxides; and
3. as a permeable support, it acts as the only solid
material in the furnace that supports the iron-
bearing burden and provides a permeable matrix
necessary for slag and metal to pass down into the
hearth and for hot gases to pass upwards into the
Of these three roles, the first two can be substituted
by oil, gas, plastics, and coal. These are injected at the
tuyeres as generating energy and a carbon source.
Such a substitution brings about a reduction in coke
rates for the blast furnace (coke rate is the weight of
coke required to produce 1 t of iron). However, there
is no other satisfactory material available, which can
replace, fully or partially, metallurgical coke as a
permeable support of blast furnace charge.
0166-5162/02/$ - see front matter D 2002 Elsevier Science B.V. All rights reserved.
PII: S0166 -5162 (02 )00123 -4
* Corresponding author. Tel.: +34-985-2808-00; fax: +34-98-
E-mail address: [email protected] (M.A. Dıez).
International Journal of Coal Geology 50 (2002) 389–412
Over the last few decades, due to ironmaking trends
towards increased size and throughput of blast furnace
performance together with a simultaneous reduction in
coke rate by high levels of injection of carbon via the
tuyeres, in particular pulverized coal injection (PCI),
the role of coke as a permeable support became greater
in importance and so further improvements in coke
quality are required. In such conditions, a decrease in
coke rate produces a decrease in the thickness of the
coke layer in the stack and cohesive zone together with
an increased residence time of coke in the lower part of
the blast furnace. Coke residence times increase by
more than 30% with variations in coal rate from 100 to
200 kg t� 1 hot metal (Negro et al., 1996). This means
that coke is subjected to longer periods under mechan-
ical, thermal, and chemical stresses that further increase
coke degradation in the blast furnace.
As a result, future research is focused to improve
these critical quality parameters of coke to reach
higher productivities when higher levels of fuel injec-
tants are operative.
A realistic assessment of the likely performance of
coke in the blast furnace operating with or without
injection technology should include those properties
of coke that reflect its resistance to degradation under
the chemical and thermal environment of the blast
furnace. Such properties, providing guidelines for
coke use, relate to lump size, shape and size uni-
formity, chemical composition, mechanical strength,
and thermal and chemical stabilities. Thus, coke for
the blast furnace needs to be a successful compromise
between structure and properties. To ensure good blast
furnace performance, coke should be moderately
large, with a narrow size range, and have a high
mechanical strength in order to withstand the weak-
ening reactions with carbon dioxide and alkali, abra-
sion, and thermal shock in the blast furnace. Because
of the many unknown factors, it is not achievable to
establish universal quality indices common to all blast
furnaces, although typical specifications for metal-
lurgical coke quality are available.
Impurities present in coke affect its performance in
the blast furnace by decreasing its role as a fuel in
terms of amounts of carbon available for direct and
indirect reduction roles and also its role as a perme-
able support. Such impurities are moisture, volatile
matter, ash, sulphur, phosphorous, and alkali contents.
Their levels are kept as low as possible.
Moisture content is a direct consequence of the
coke-quenching process with some dependence on
size. High and variable moisture contents affect both
the coke rate and the balances within the blast furnace,
while high volatile matter contents cause operational
problems in the cleaning of blast furnace gas. Coke
moisture content ranges from 1 to 6 wt.% maximum
and common values are in the range 3–4 wt.%.
Of other chemical properties, sulphur and ash
(content and chemistry) are of particular importance
because as they increase, coke productivity in the
blast furnace decreases. The coke ash is a non-
productive part of coke which influences slag volume
and composition. Industrial experience indicates that a
1 wt.% increase of ash in the coke reduces metal
production by 2 or 3 wt.%. Values higher than 10
wt.% can be satisfactory but only if the ash chemistry
Recent papers summarize coke quality require-
ments for some operating blast furnaces in Europe
(Leonard et al., 1996; Großpietsch et al., 2000) with
typical coke chemical properties being given in
The importance of coke physical properties is
linked to the need to support the ferrous burden and
to give a permeable matrix through which reducing
gases can flow and molten material can percolate in
the lower blast furnace region. These physical proper-
ties are related to its size (mean and distribution) and
its resistance to breakage and abrasion. Coke size is
mostly controlled by screening. A large mean size
with a narrow size distribution maintains adequate
permeability. Most operators consider a mean opti-
mum size to be in the range of 50–55 mm.
Empirical mechanical strength tests, commonly
used to measure resistance to size degradation, involve
Required chemical properties of blast furnace coke (Leonard et al.,
Chemical property European range
Moisture (wt.%) 1–6
Volatile matter (wt.% db) < 1.0
Ash (wt.% db) 8–12
Sulphur (wt.% db) 0.5–0.9
Phosphorous (wt.% db) 0.02–0.06
Alkalies (wt.% db) < 0.3
db = dry-based.
M.A. Dıez et al. / International Journal of Coal Geology 50 (2002) 389–412390
dynamic loading either in the form of shatter tests
(ASTM D3038), where breakage occurs by impact; or
revolving drum tests such as ASTM Tumbler (ASTM
D3402), MICUM, half- and extended-MICUM, IRSID
and JIS (JIS K2151) tests, where attrition takes place
by a combination of breakage and abrasion. In Europe,
the MICUM and IRSID (ISO 556 and ISO 1881) tests,
which use the same equipment, are dominant. Details
of these tests have been reported elsewhere (Patrick
and Wilkinson, 1978; Ragan and Marsh, 1980; Loison
et al., 1989; Alvarez and Dıez, 2000).
Highly stabilized blast furnace coke needs a high
abrasion resistance. The range of optimum values,
however, is wide and strongly dependent upon the
characteristics and operational conditions of the blast
furnaces. As an example, typical coke size and
strength values for European blast furnaces are given
in Table 2 together with those reported for current
operation in Australian BHP Port Kembla, American
and Japanese blast furnaces.
Although coke mechanical strength indices provide
blast furnace operators with a useful assessment of
coke performance, they form only part of the overall
picture. The tests used to assess coke mechanical
strength are made at ambient temperature and hence
fail to take into account the process conditions of the
coke in the blast furnace.
The importance of high temperature properties of
coke was established by the Japanese Steel Industry
from the dissection surveys of three blast furnaces that
were quenched whilst operating (Nakamura et al.,
As a result, a combined test for measuring the coke
reactivity and post-reaction strength was introduced by
the Nippon Steel Corporation (NSC) in the 1970s. The
NSC method is described in a research report pub-
lished by The British Carbonization Research Associ-
ation (BCRA) (1980). Recently, it has been adopted as
an ASTM standard procedure (ASTM D 5341-93a)
and is currently being prepared by the International
Organization for Standardization (ISO). The method, a
major coke quality test which has achieved interna-
tional routine use by industry, measures the solution
loss reaction of coke by carbon dioxide at 1100 jC for
2 h (Coke Reactivity Index—CRI) under standardized
gas flow rate conditions together with the coke
mechanical strength after reaction with carbon dioxide
(CSR index). For a good quality coke, the CRI should
be low and the CSR index high. If the coke reacts
excessively with the oxidizing gases of the blast
furnace which contain increasing proportions of car-
bon dioxide, coke will weaken and will be degraded
into smaller particles. Excessive coke degradation
leads to permeability reduction, impaired efficiency
of blast furnaces performance, and blockage of the
tuyeres with coke residues. A high degree of correla-
tion between the two indices, CRI and CSR, derived
from the NSC method was found by various authors.
Fig. 1 shows, as an example, the relationship between
Required physical properties of blast furnace coke in current
Mean size (mm) 47–70 50 50 45–60
M40 ( + 60 mm) >78–>88 85 n.a. n.a.
M10 ( + 60 mm) < 5– < 8 6.5 n.a. n.a.
I40 53–55 n.a. n.a. n.a.
I20 >77.5 n.a. n.a. n.a.
DI150/15 n.a. 84.4 n.a. 83–85
ASTM stability n.a. 63.6 60 n.a.
CSR >60 74.1 61 50–65
CRI 20–30 17.7 23 n.a.
Data taken from: aLeonard et al., 1996 (also in Großpietsch et al.,
2000);bHorrocks et al., 2000; cPoveromo, 1996; O’Donnell and
Poveromo, 2000 (data presented from AISI coke quality survey) anddNishioka, 2000.
n.a.: not available.
Fig. 1. Relationship between CRI and CSR indices (after Menendez
et al., 1999).
M.A. Dıez et al. / International Journal of Coal Geology 50 (2002) 389–412 391
CRI and CSR index for a series of more than 60 cokes
produced from single coals of different rank and geo-
graphical origin and from complex coal blends
(Menendez et al., 1999). The cokes were produced at
the INCAR Experimental Coking Test Plant (Dıez et
al., 1991) using a coke oven of 6-t capacity in
operation until July 1999. A correlation exists between
CRI and CSR indices derived from the NSC test, but
some points show scatter, being greater for high re-
active cokes. Based on such a relationship, one param-
eter should be sufficient to classify a coke and, then,
the CSR index is commonly used in the control of
quality of blast furnace coke.
Other tests developed to evaluate the coke reac-
tivity are summarized in a recent publication (Menen-
dez et al., 1999). These authors show a correlation
between the ECE-INCAR reactivity and the CRI and
CSR indices for 33 different cokes (r2 = 0.9463 and
0.9339, respectively). The ECE-INCAR method
measures metallurgical coke reactivity and is based
on a test standardized by the United Nations Eco-
nomic Commission for Europe (UNECE) (1965). In
this test, a smaller amount of coke (7 g) with smaller
particle size (1–3 mm) in comparison to the NSC
test, which uses 200 g of coke of 19–21 mm size, is
Several authors have demonstrated the relevance of
CSR in blast furnace operation to maintain perme-
ability at constant and optimum values. For instance,
it was found that when the CSR index decreases, the
gas permeability resistance or impermeability index
increases (Nakamura et al., 1977; Hatano et al., 1990;
Colleta et al., 1990). From these relationships, differ-
ent minimum values of CSR indices have been
established to ensure stable operation, i.e., CSR values
>48% and >55% for coke feed at NSC Oita and
Kimitsu blast furnaces, respectively. A CSR index
higher than 58%, needed to achieve an impermeability
index lower than 6, was established at the Taranto
works in Italy (Colleta et al., 1990). Moreover, due to
a better burden permeability, an increase in CSR of
1% in the specific CSR range 45–55% accounted for
1.5 kg t� 1 reduction in fuel rate in the NSC Hirohata
works (Hara et al., 1980). For a Port Kembla blast
furnace, an increase of 30 t day� 1 in iron output and a
fall of 0.4 kg t� 1 in fuel rate for CSR, in the ranges
52–62% and 58–73%, respectively, is also reported
by Rooney et al. (1987).
More so, the largest blast furnaces, operating with
low coke rates (high PCI levels) and high productiv-
ity, also showed the importance of high CSR indices.
Experience shows that with increasing CSR index of
coke feed to the larger blast furnaces, the injected coal
level can be increased and the low coke rates main-
tained. However, CSR indices below 60%, in most
cases, are not acceptable because of resultant higher-
pressure losses and reduced furnace permeability
(Großpietsch et al., 2000). CRI indices should be in
the range of 20–30%.
Despite the beneficial effects of a high CSR of
coke on blast furnace operation and fuel consumption,
some doubt has been raised about the validity of the
experimental conditions related to the CRI and CSR
measurements (Vogt, 2000). Some blast furnaces, for
instance, operate stably with low CSR cokes. Coke in
the blast furnace is subject to varying temperatures
and gas compositions. Gasification occurs in the
presence of many other reactions, some of them are
interactive principally the reduction of the iron ore.
However, no other test today has reached an industrial
application. Assessment of coke quality using CRI
and CSR indices, as defined by NSC, dominates in
As with other coke quality parameters, there is no
single optimum value of CSR and CRI. It may vary
between blast furnaces having different furnace char-
acteristics and operational conditions but having the
same coke rate. Coke qualities used by different
European Companies are reported in Joint European
Blast Furnace Committee papers presented at the two
last European Cokemaking–Ironmaking Conferences
(Leonard et al., 1996; Großpietsch et al., 2000).
Typical coke quality values are in Table 2 together
with those reported by non-European producers (Hor-
rocks et al., 2000; Poveromo, 1996; O’Donnell and
Poveromo, 2000; Nishioka, 2000).
An interesting aspect of the joint European Coke
Committee paper presented at the 3rd International
Cokemaking Congress is the estimation of the max-
imum attainable coke quality based on actual coking
plant data (Vander et al., 1996). For a coke with a
stabilization of a 25-m drop, the CRI and CSR
estimated values are 24% and 70%, respectively, for
a conventional coke oven of 450-mm width operating
with a coking time of 18 h. These coke quality
parameters can be achieved for coal blends develop-
M.A. Dıez et al. / International Journal of Coal Geology 50 (2002) 389–412392
ing a maximum gas pressure of about 7 kPa. Major
limitations to obtain higher coke quality are consid-
ered to be coking pressure and the conventional
coking process itself. Analysis of operating results
by NSC in the 1970s suggested that CSR depends
about 70% on the coal or coal blend and about 30%
on coking conditions (Nakamura et al., 1977). The
importance of the coal blend as a factor in coke
gasification has been noted by other researchers
(Bernard et al., 1985, 1986). Although coking con-
ditions, for example, bulk density, coking time, pre-
heating of the charge, and the incorporation of non-
coal materials, do minimize some deficiencies in coal
properties, the selection of an optimum coal or coal
blend is a priority for best coke.
2. Coke structure and its effects on coke properties
Over the past 30 years, an extensive literature
describing relationships between coke structure and
properties has been generated. This paper does not
review these papers but reports general guidelines.
There is a close relationship between the CSR
index and the vitrinite reflectance of coal. The CSR
index passes through a maximum in the region of
prime coking coals with mean reflectance of 1.2% to
1.3% and falls towards coals of lower or higher rank
(Nakamura et al., 1977). Fig. 2 shows the relationship
of CSR index with coal rank. As coke reactivity to
CO2 is inversely related to CSR, there are minimum
values of reactivity to CO2 in the region of prime
coking coals, increasing for cokes from lower and
higher rank coals (Hyslop, 1981; Patrick and Wilkin-
son, 1981). Such a behavior may be explained by the
relative proportion of the different structural compo-
nents within coke with strong dependence of coal
rank. However, some cokes fall outside this close
relationship (Hyslop, 1981), indicating that rank,
although being a dominant factor, is not the only
factor that influences CRI and CSR. Catalytic effects
of the coke gasification and coking conditions also
need to be considered (Fig. 3).
It is established that the rank and chemistry of the
parent coal strongly influence the optical textures of
cokes. Several studies show that the development of
anisotropy (size, shape and intensity) during carbon-
ization varies mainly with (a) coal rank; (b) petro-
graphic composition of the coals; (c) plasticity of the
parent coal; (d) carbonization conditions such as rate
of heating, soak time and gas overpressure; as well as
(e) the nature of additives used in the coal blends
(Marsh, 1982, 1992; Marsh and Clarke, 1986).
In recent years, fundamental research has demon-
strated that metallurgical coke should be considered as
a composite material whose strength and reactivity
depend on contents of isotropic carbon and inerts, the
size and shape of the anisotropic carbon units, and the
interfaces between textural components together with
porosity and ash chemistry (Marsh and Clarke, 1986).
Coke strength involves fissuring and breakage
along the boundaries of, or sometimes through, both
macroscopic and microscopic coke components, with
porosity being a dominant factor (Patrick and Walker,
1995). For cokes of comparable porosities, differences
Fig. 2. Relationship between vitrinite reflectance and coke strength
after reaction with carbon dioxide (CSR index) (Nakamura et al.,
Fig. 3. Main factors influencing the coke strength after reaction with
carbon dioxide at 1100 jC (CSR index).
M.A. Dıez et al. / International Journal of Coal Geology 50 (2002) 389–412 393
in strength and related properties are dependent upon
the constituents of pore-wall material. Marsh and
Clarke (1986) summarized the following considera-
tions about the strength of optical textural components
and the strength of binding at the interface: (a)
mosaics are interlocked with each other at the molec-
ular level to form a firmly bonded interface; (b) fissure
propagation across the randomly orientated mosaics is
not facilitated by this type of structure; (c) inert
materials in coke coming from both the parent coal
or added breeze coke may either be encapsulated if
they have smooth surfaces or may be interlocked over
rough or porous surfaces; and (d) coke microstrength
increases with coal rank to a maximum as the struc-
ture of the coke changes from isotropic, to mosaic,
and to flow-type anisotropy.
To this end, a methodology has been developed to
quantify the degree of bonding in the transition zones
between the textural components of coke and the
binding between textural components and inert mate-
rial interfaces (Barriocanal et al., 1994). Coke proper-
ties and coking behavior of single coals and blends
using petroleum coke (Menendez et al., 1996, 1997)
and waste materials (Barriocanal et al., 1998) have
been related to extent of bonding at interfaces between
optical textural components and inert material. Con-
cerning coke reactivity, significant progress has been
made in the understanding of those factors controlling
internal bonding of cokes such as the coal rank,
amounts of inerts and ash in coal, the metal oxide
content of coke ash, and the optical textural compo-
nents of the coke. Optical microscopic observations
on non-gasified and gasified cokes established a
relative reactivity scale for the different components
in coke, inert>isotropic>fine mosaic>coarse mosaic>
flow (Fujita et al., 1983).
3. Coke quality prediction
Currently, normal practice in cokemaking demands
a coal blend that is low in cost, produces a high
quality coke, and provides a safe oven pushing
performance. Coal blending has been adopted by the
industry partially because of the limited availability
and high cost of prime coking coals and also because
of the continued demand for better quality coke for the
blast furnace. Coal blending varies in the number of
coals used (four or more), the proportion, rank, coking
properties, and geographical origin of coal compo-
Coal selection and blend composition are major
factors controlling coke properties (physical and
chemical). As aids to coal selection and coke quality
prediction, several mathematical models are available,
divided into two groups according to the coke proper-
ties involved. The first-generation group of models
focuses on the prediction of cold mechanical coke
strength (i.e., ASTM stability and MICUM indices).
The second-generation of models uses the CRI and
CSR indices as coke quality parameters. As far as can
be ascertained, no prediction model has reached
universal application. Some coals or blends show
significant deviations between values predicted by a
model and values obtained experimentally. However,
almost all coking plants have, for internal use, some
form of a model based on coal rank, rheological
properties, petrology, and ash chemistry.
3.1. Prediction models of coke strength from coal
Strength is the most important physical property of
coke with considerable effort attempting correlations
with coal rank and type in terms of total inert content,
rheology as indicated by maximum fluidity, total
dilatation, and parameters deduced from petrographic
compositions of coal. Based on these considerations,
some mathematical models use petrographic compo-
sitions in the evaluation of the coal coking potential
and the prediction of coke strength. Thus, petro-
graphic analyses are assuming a major role in coal
Petrographic analyses for the prediction of coking
properties have classified macerals into reactives and
inerts. The pioneering works of Stopes (1919) pro-
vided the basis for a definition of coal composition
based on the optical properties and the ‘‘maceral
concept’’ (Stopes, 1935). This represented a major
advance into understanding of how an optimum ratio
of reactive and inert components affects coal carbon-
ization properties and behavior. The term ‘‘reactives’’
includes those macerals which soften on heating and
bind ‘‘inerts’’ (those macerals that remain unaltered on
heating) and then resolidify into a porous, fused, solid
carbon material. Consequently, coke structure should
M.A. Dıez et al. / International Journal of Coal Geology 50 (2002) 389–412394
be considered as a composite material where most of
the coke constituents came from the reactive materials
(binder) and a much lower proportion from the
material which acts as a filler (inerts) during the
carbonization process. To obtain a good coke, a
known proportion of reactive and inert material is
required and the optimum amount of each one will
vary with the type of reactive macerals. In general,
reactive macerals include vitrinite, liptinite, and one-
third of semifusinite, while inert coal constituents
during carbonization are two-thirds of semifusinite,
fusinite, macrinite, micrinite, inertodetrinite, sclerotin-
ite, and mineral matter (Ammosov et al., 1957;
Schapiro and Gray, 1960). However, such a classifi-
cation of coal reactive and inert constituents is not
equally applicable to all coals, consequently some
laboratories do not follow it in detail. In particular,
the division of the amount of semifusinite acting as
reactive or inert is controversial. An explanation for
this discrepancy is that composition and, hence,
technological behavior of some macerals may differ
from region to region because of different coalifica-
tion and depositional conditions causing, e.g., for one
coal to contain macerals that are mainly inert but
which are reactive in another coal. Thus, Benedict et
al. (1968a) considered a similar breakdown for semi-
fusinite plus other inertinite macerals of low reflec-
tance, while other authors used little semifusinite in
their reactives (Brown et al., 1964); or relatively large
and variable amounts (Steyn and Smith, 1977).
More details on the development on coal petrology
(classifications and behavior of maceral groups and
microlithotypes and its application to cokemaking)
have been published in a number of excellent reviews
(Stach et al., 1982; Bustin et al., 1985; Falcon and
Snyman, 1986; Kaegi et al., 1988). As an introduction
on coal petrology, a recent book chapter also summa-
rizes the work carried out on this area (Suarez-Ruiz,
Based on the maceral behavior during carboniza-
tion (reactive and inert), a concept that is used today
for explaining coal carbonization behavior, several
mathematical models have been developed to predict
coke strength. Each model seems to estimate with a
high degree of accuracy when they are applied to
coals which are more or less similar in petrographic
composition to the coals for which the model was
developed, and coke potential is being evaluated on
coals which might be tested under the same exper-
imental conditions used in the model.
Two models were developed in USA based on
petrographic data for the prediction of coke strength
and the formulation of coking blends, one developed
by United States Steel and the other by Bethlehem
Steel. A detailed history of the development of the
two models has been recently reported (Dutcher and
Crelling, 2000; Spackman, 2000; Thompson, 2000).
The US Steel model for ASTM coke stability was
firstly designed by Schapiro et al. (1961) and based on
the earlier Russian work of Ammosov et al. (1957).
The model of Ammosov et al. (1957) relates to coke
prepared in commercial coke oven batteries and
predicts coke strength from the petrographic data of
the parent coals. Schapiro et al. (1961) modified this
model and applied it to coals used by US Steel for the
prediction of the ASTM stability factor. Schapiro and
Gray (1964), and later Harrison et al. (1964) and
Moses (1976), further developed the models. The
US Steel model is the basis for predicting coke quality
from specific coals. The reactive coal components
include all vitrinite and liptinite and one-third of the
semifusinite, while the inerts include the remaining
two-thirds of the semifusinite, together with the
remaining inertinite and mineral matter. This model
requires data from the maceral and reflectance analy-
ses in which the reflectance of all the reactive and
semi-inert macerals are measured, as well as the
calculation of mineral matter of coal (MM) by the
Parr formula (MM=1.08 Ash + 0.55 Spyritic (Loison et
al., 1989, p. 29)). Reactive macerals are further sub-
divided into 21 ranges of 0.1% reflectance (vitrinoid
type, V-type). From petrographic data and coke
strength values, different curves can be plotted: (a)
the optimum ratio of reactives to inerts (R/I) for each
vitrinoid type; (b) the variation of the strength index
(SI) with the quantity of inerts for various vitrinoid
types; and (c) the variation of the strength index with
the composition balance index (CBI) for various
stability factors. For each vitrinoid type (V-type),
there is an optimum ratio of reactive to inert compo-
nents that influences maximum coke strength (opti-
mum inert ratio). This optimum inert ratio was
established by physically isolating each of the macer-
als and determining, by means of micro-coking tests,
what ratio gave the maximum strength value. With
higher or lower proportions of inerts than the opti-
M.A. Dıez et al. / International Journal of Coal Geology 50 (2002) 389–412 395
mum, the coke strength decreases. The other indices
defined by these authors are: a composition balance
index (CBI) and a strength index (SI), the latter also
being referred to as a rank index. CBI is the ratio of
inert components in coal to the optimum ratio of
reactive to inert that a coal of a given rank should
have. When for a given coal the optimum CBI is equal
to 1, the best coke is obtained. The strength index (SI)
can be evaluated to determine the relative coke
strength made from coals of different ranks and types.
Thus, it is possible to predict ASTM stability factors
from CBI (as a caking property parameter) and SI (as
a rank parameter).
An advantage claimed for this model is that both
indices, CBI and SI, are additive and it should be
possible to use petrographic assessments without pilot
coke oven tests. The US Steel model gave fully
satisfactory results for the low semifusinite Appala-
chian coals and blends for which the system was
developed. However, this model is based on correla-
tions of test-coke data with the petrographic compo-
sition of the coals being carbonized, keeping the test
conditions constant. The restrictions of this model are
limited to a < 2 wt.% of moisture content of coal, ash
content no higher than 12 wt.%, tested coals crushed
to 80 wt.% minus 1/8 in. in size, the bulk charge
density of approximately 55 lbs/ft3, and a coking rate
of 1 in. per h (note: 1 in. = 2.54 cm).
Various coke prediction models, in general, follow
the same approach of Schapiro et al. (1961). The
Bethlehem Steel model, first reported by Benedict et
al. (1968a) and later by Thompson and Benedict
(1976), was developed to accommodate the Eastern
Kentucky coals used in coal blends of this company.
Similarities are related to the use of a one-third–two-
thirds breakdown of semifusinite and other semi-
inerts, and the use of maximum reflectance as the
parameter of rank determination. Differences with
Schapiro et al. (1961) are mainly concerned with the
carbonization behavior of that part of the vitrinite
maceral group that remains unaltered in the coke. They
called this material pseudovitrinite (Benedict et al.,
1968b). The inertness of pseudovitrinite is determined
by: (a) separate measurements of the maximum reflec-
tance on pseudovitrinite (RmaxPsv) and normal vitrinite
(Rmax); (b) the reflectance spread (RmaxPsv�Rmax);
and (c) estimation of the pseudovitrinite amount that
should be included in the effective inert content. The
remaining pseudovitrinite is considered to be a reactive
component. The ASTM stability factor can be esti-
mated from the effective inert content and the normal
This petrographic model has been adapted to select
coals not having excessive coking pressures (Benedict
and Thompson,1976). Some low-volatile coals, espe-
cially those with vitrinite reflectance >1.65% and of
low inert content, produce excessively dangerous
pressures during carbonization (Tucker and Everitt,
1992). In normal industrial practice, these low-volatile
coals are never coked singly and are normally used as
a 25–30 wt.% component in coal blends. The authors
showed that both, vitrinite reflectance and maceral
composition of coal, could be related to excessive
pressures during carbonization. Coking pressure var-
ied directly with reflectance and inversely with effec-
tive inert content of low-volatile coals. The model
allows a classification of coals as safe, marginal and
The coke strength prediction model of Brown et al.
(1964) differs from those already described in the
subdivision of semifusinite. They considered that
‘‘virtually all semifusinite remains unchanged during
carbonization and the same applies to micrinite’’. The
predominant inert character of semifusinite was first
noted by Taylor (1957) who concluded, ‘‘semifusinite
may be distorted and altered in its chemical nature,
but that no appreciable amount fuses and enters the
fused coke structure’’. Taylor et al. (1967), in an inter-
laboratory study, provided evidence of the inert role of
semifusinite using a range from low volatile to high
volatile bituminous coals. They also suggested that
transitional material between vitrinite and semifusinite
became weakly plastic during heating and it should be
included in the category of vitrinite. Consequently,
they suggested that, as a rule, semifusinite with a
reflectance higher than 0.1 to 0.2 compared with the
mean reflectance of vitrinite in the same coal is inert.
Other authors argued that the inert character of the
semifusinite could be a result of the small laboratory-
scale test oven, used in the carbonization tests. In
coking conditions, the semifusinite could be much
Brown et al. (1964) considered two other factors
not already applied in the models previously
described. One is related to the dimensions of the
inertinite material in the coal. If the inertinites are
M.A. Dıez et al. / International Journal of Coal Geology 50 (2002) 389–412396
relatively large, they tend to form centers of weakness
in the resulting coke and therefore have a deleterious
effect on strength. The second factor concerns the
relative association of reactive and inert materials. For
these reasons, a prediction of coke quality (shatter
index and ASTM hardness factor) using Australian
coals was undertaken in terms of the microlithotypes,
vitrite and clarite. The method can provide useful
information on coke strength to assess the potential
of a given coking coal.
On the other hand, when Cretaceous coals from
Western Canada, with a higher proportion of semi-
fusinite than Carboniferous coals were used, the
model of Schapiro et al. (1961) predicted coke
strength values lower than those measured experimen-
tally. To get satisfactory coke strength prediction
using such coals with a total semifusinite content
greater than 20%, CANMET introduced a modifica-
tion based on the assumption that semifusinite makes
a greater contribution to the reactive components
(Carr and Jorgensen, 1975). They decided that half
of the semifusinite is effectively a reactive component.
However, no evidence was found to support this
assumption. The work of Nandi and Montgomery
(1975) on the nature and thermal behavior of semi-
fusinite in such coals using a hot-stage microscope
provided useful data. They concluded that high-reflec-
tance semifusinite is a totally inert component during
carbonization (no signs of melting or softening were
observed at 450 jC), while low-reflectance semifu-
sinite was reactive, similar to vitrinite, and its melting
point being about 85 jC lower than that of the
corresponding vitrinite. The pure vitrinite was melted
at a temperature of 420 jC.Based on these conclusions, other models devel-
oped for CANMET (Pearson and Price, 1985) intro-
duced the ‘‘cut-off’’ reflectance or reactive ‘‘cut-off’’
value (Rcut-off) that separates reactive and inert mac-
erals in a random reflectogram of all coal macerals. A
good correlation between maximum vitrinite reflec-
tance and Rcut-off for 76 coals ranging from 0.89% to
1.63% (Rmax) was found (r2 = 0.92). For a given coal,
the new parameter can be deduced from the correla-
tion between Rmax and Rcut-off.
Recently, the proportion of semifusinite as a reac-
tive component, in the range of 33–50%, has been
determined by coke microscopy. The proportion
varies from coal to coal and 50% of the reactive
semifusinite is recommended for Western Canadian
coals when coal petrography is used to predict coke
strength for blends. Another problem is to explain the
low rheological values for Western Canadian coals.
The rheological values cannot be compared to other
similar rank coals (Australian or US Carboniferous
coking coals) and, therefore, they should not be
directly used in calculations of average fluidities of
blends containing coals from many sources (Leeder et
al., 1997). High quality coke can be produced from
Canadian coals with maximum fluidities in the range
of 3–10 ddpm. These values strongly differ from the
minimum value of maximum fluidity (100–200
ddpm, see below) established in the MOF diagram
(relation between Gieseler maximum fluidity and
maximum reflectance of vitrinite for coal blending
used in Japan). On the other hand, comparing dilata-
tion values of Canadian and US coals of the same rank
and inert content, Canadian coals have a total Ruhr
dilatation of approximately three to four times lower.
The authors suggested two approaches to assist with
coal blend preparation. One is to use an ‘‘equivalent’’
maximum fluidity for blends containing low propor-
tions of Canadian coals. However, it is concluded that
the most satisfactory evaluation of the influence of
such coals in blends made with coals from other
sources is the use of pilot-scale carbonization tests.
Another prediction model is that developed by
Steyn and Smith (1977) from ISCOR in South Africa.
In this model, variable proportions of semifusinite as
reactives are considered. Many South African coals
have relatively low vitrinite contents and large
amounts of semifusinite and of micrinite. With such
coals, the coking coal blend is characterized by a
similar amount of vitrinite and semifusinite plus
micrinite. For instance, vitrinite contents are as low
as 40% and semifusinite and micrinite contents are as
high as 45%. Both semifusinite and micrinite should
have a significant role during carbonization and for
technological purposes need to be classified according
to reflectance and structure into reactive and inert
types. The authors indicated that ‘‘the classification
proposed complicates maceral analysis but elucidates
the coking behavior of low-vitrinite coals’’.
Other models to predict coke strength do not
exclusively use coal petrography and utilize the dila-
tation characteristic of coals and blends using a Ruhr
or Audibert-Arnu dilatometer. The model devised by
M.A. Dıez et al. / International Journal of Coal Geology 50 (2002) 389–412 397
Mackowsky and Simonis (1969) in Germany provides
not only a basis for prediction of the MICUM strength
and abrasion indices (M40 and M10) for cokes pro-
duced from a range of Ruhr coals and blends, but also
yields of carbonization products (coke, gas, liquid by-
products, and tar). In addition to coal composition
parameters, the model takes into account coking
conditions, that is, coal size of the charge, bulk
density, coking rate, mean oven width, and coking
In this model, the MICUM M40 index (wt.% of
coke, >40 mm after 100 revolutions) is expressed as:
M40 ¼ aK þ bþ dMs
Where K is a factor including the coking conditions as
a function of the bulk density, oven width and coking
time; Ms is the particle size content of the coal; b is a
rank factor; and a and d are coefficients based on
volatile matter and a parameter named G-factor.
The G-factor is usually obtained from parameters
derived from the Ruhr dilatometer test, which is a
modification of the Audibert-Arnu dilatometer test
(the softening and resolidification temperatures and
the percentage of coal contraction and dilatation).
Although the G-factor is considered additive for coal
blends, there is a limitation for blends composed of
coals whose plastic range does not overlap sufficiently
(Gibson, 1972). Experiments on the behavior of the
different maceral groups in this dilatometer showed
that it was also possible to calculate the G-factor for a
given coal from its petrographic composition.
The prediction model for M40 and M10 indices
(wt.% of coke >40 mm and < 10 mm in size, respec-
tively, after 100 revolutions) can only be applied to a
certain range of coals characterized by volatile matter
contents between 18 and 35 wt.% daf and inert con-
tents below 20%, this being very restrictive.
A quite different approach to predict coke strength
is based on the relationship between petrographic data
(Rmax) and rheological properties (Gieseler maximum
fluidity) of the coals (MOF diagram). The fundamen-
tal concept for the blending target used is based on the
assumption that coke strength is mainly governed by
two main coal properties, i.e., the caking property and
the rank of coal. Fig. 4 shows the dominant regions
for each parameter.
The model developed by Nippon Kokan (NKK) in
Japan is described as a coal property ‘‘window
model’’, where the blending ratio is determined such
that the maximum vitrinite reflectance and maxi-
mum fluidity of the coal blend falls within an
established optimum range (‘‘window’’ or ‘‘rectan-
gle’’). If the coal blend characteristics fall inside this
window, the resulting coke will be of acceptable
quality for blast furnace use (Okuyama et al., 1970;
Miyazu, 1974; Miura, 1978). Within the framework
of this model, desirable properties of a coal blend
range of 1.2–1.3% and a Gieseler maximum fluidity
between 200 and 1000 ddpm (Fig. 5). The coal
blends must meet these specifications if the target
coke strength index of higher 92.0 (JIS DI30/15,
wt.% of 15 mm coke after 30 revolutions) is to be
To determine the role of each coal in the blend, the
MOF diagram (Fig. 5) is divided into four quadrants.
Coals belonging to quadrants I and II provide
adequate fluidity to the blend, while coals within
quadrant IV are used to adjust the rank of the blended
coals. However, coals with both low rank and low
fluidities (in quadrant III) are used only as a source of
carbon for blending.
The ‘‘window’’ of acceptable blends defined from
the MOF diagram has been regarded as being too
restrictive by the Centre de Recherches Metallurgiques
(CRM) in Belgium. Here, blends with the optimum
characteristics described in the MOF model (falling
within the ‘‘window’’) gave excellent coke strength.
Fig. 4. Diagram showing the dominant regions of the fluidity and
the rank of coal to control coke strength (Miura, 1978; Morishita et
M.A. Dıez et al. / International Journal of Coal Geology 50 (2002) 389–412398
However, blends located outside of the optimum win-
dow also gave high quality coke indices (Poos, 1987).
For the coal blends studied, other prediction models do
not work satisfactorily. The CRM has developed a coke
strength prediction model based on three parameters:
(a) the inert content of coal, (b) the reactive caking
index, and (c) the maximum fluidity (Munnix, 1984).
The reactive caking index was defined as a function of
vitrinite reflectance. Formulae have been developed for
calculating each of these parameters for blends from the
values of the individual coals carbonized in a 300-kg
Modifications to the Japanese MOF diagram were
introduced by Spanish Steel, Ensidesa (now, Acera-
lia), to accommodate coal blends used for coke
production (Sirgado and Verduras, 1978). For better
correlation of coal rank with coke strength, they
defined the mean effective reflectance of vitrinite as
the mean random reflectance of vitrinite restricted to
the range of V-steps 6 to 18 (both included).
The Coal Research Establishment in UK estab-
lished a target specification for the blending of high-
and low-volatile coals based on total dilatation and
volatile matter content (Gibson, 1972; Gibson and
Gregory, 1978). It is recognized that these two param-
eters, generally, are not sufficient in themselves. In
addition, it is necessary to consider the size distribu-
tion of the mineral matter associated with the coal and
the compatibility of blend components.
In summary, because of the fundamental publica-
tions by Ammosov et al. (1957) and Schapiro et al.
(1961), the prediction models of coke strength have
expanded considerably. Noting that coke quality
parameters are strongly dependent on coal properties,
efforts were focused on the use of petrographic and
rheological properties. With regard to the single coal
and coal blends used, one prediction model can be no
better than any other model. That is, it is satisfactory if
the model is confined to a particular coal and coal
blend. Its application to coals of different geological
histories is less successful.
3.2. Prediction models of CRI and CSR indices
In the first-generation group of models, coking coal
properties were mostly established by petrographic
and rheological properties in order to predict cold
mechanical strength of blast furnace coke. But, many
coal deposits having excellent coking ability from a
traditional point of view, do not have an acceptable
mineral composition. After introducing the parameters
CRI/CSR to assess coke quality, the role of the ash
composition has been given more consideration
because certain minerals in coke have an accelerating
or inhibiting effect on coke gasification because of
catalytic reactions. From the almost linear correlation
between CSR and CRI indices, it is deduced that the
lower the reactivity the higher the coke strength (Fig.
1). Then, catalytically accelerated coke reactivity lead
to lower CSR values even if the coking coal blend has
excellent rheological properties. Fig. 3 summarizes the
factors affecting the CSR and used in prediction
models. Taking into account the above considerations,
from the adoption of the NSC model for testing coke
quality, different approaches have been developed for
predicting the CRI and CSR indices and continue to be
a research subject of considerable interest. They can be
considered to be second-generation prediction models.
Fig. 5. Relationship between Gieseler maximum fluidity and
maximum reflectance of vitrinite for coal blending target (MOF
diagram) (Miyazu, 1974).
M.A. Dıez et al. / International Journal of Coal Geology 50 (2002) 389–412 399
On this topic, excellent reviews exist in the literature
(Goscinski et al., 1985; Goscinski and Patalsky, 1990;
Valia, 1989; Gransden et al., 1991; Edwards, 1991).
The first attempt to predict CSR from coal proper-
ties was made from the mean vitrinite reflectance and
the inert content (Miura, 1978). Following that, differ-
ent prediction models from coal properties have been
reported by several authors.
The model developed by NSC is based on the
vitrinite reflectance and the inert content of coal,
including inertinite plus two-thirds of semi-inertinite.
Similar to the approach of Schapiro et al. (1961) for
predicting ASTM stability factor, an optimum inert
content for each vitrinite reflectance is necessary to
obtain the best CSR value (Hara et al., 1980). They
suggest that as CSR is controlled at least in part by the
previous CO2 gasification, an important role may be
also expected of the ash content and composition.
Further studies on coals, prepared by ‘specific
gravity’ separations, with the same mean vitrinite
reflectance, but containing different amount of iner-
tinite and ash conclude that inertinite, especially in
coals with low reflectance, increases reactivity
towards carbon dioxide even when the coke has a
low ash content (Sakawa et al., 1982). A multi-para-
metric equation to predict reactivity towards carbon
dioxide as a function of the mean reflectance of
vitrinite, the inertinite content, and an alkali index,
including quadratic and interaction terms, has also
been reported. In this model, the rate of CO2 gas-
ification of coke is estimated as follows:
K ¼ aR2 þ bI2 þ cB2 þ dRI þ eBI þ fBRþ gR
þ hI þ iBþ j
where R, the mean reflectance of vitrinite; I, the
inertinite content; B, the alkali index; and, a– j,
numerical constants calculated from the least-squares
The alkali index (Bash) defined in this model can be
Bash ¼ ash ðwt:%Þ½ðFe2O3 þ CaOþMgOþ Na2O
þ K2OÞ=ðSiO2 þ Al2O3Þ�
The NSC model, using a multi-parameter equation,
has been used by Taranto works in Italy. For over 50
individual coals, a correlation coefficient of 0.91 was
obtained for the relationship between the estimated
values and experimental CSR values. The latter were
determined from cokes produced from single coals
placed in a box located in an industrial coke oven. A
standard deviation of residuals of 1.7% was obtained
(Colleta et al., 1990).
The model developed by Kobe Steel predicts coke
strength after reaction (CSR) by means of the Reac-
tion Strength Index (RSI), which is determined differ-
ently than the NSC model. The model, as reported in
the review papers (Goscinski et al., 1985; Goscinski
and Patalsky, 1990; Valia 1989; Edwards, 1991), is
based on mean vitrinite reflectance (R0), Gieseler
maximum fluidity (MF) expressed as logarithm (base
10), and the ratio of principal basic (Fe2O3 +CaO+ -
K2O+Na2O) and acidic (SiO2 +Al2O3) components
in the coal ash, as follows:
RSI ¼ 70:9þ R0 þ 7:8ðlog MFÞþ 89½ðFe2O3 þ CaOþ Na2Oþ K2OÞ=SiO2 þ Al2O3Þ� � 32
where CSR =RSI� 10.
A similar model for RSI prediction, later reported
by Kobe Steel (Oguri et al., 1987), differs mainly in
the basicity or alkali indices which are used. The
model takes into account previous findings which
indicate how coke reactivity is affected by: (a) textural
components in coke, which are mainly controlled by
coal rank reflected as the mean vitrinite reflectance;
(b) coke pore volume which is mainly controlled by
the development of fluidity; and (c) ash components,
especially Fe2O3 and K2O. A new basicity index
(Bash) was defined as follows (Oguri et al., 1987):
Bash ¼ ash� ðFe2O3 þ CaOþ Na2Oþ K2OÞ
However, using the new parameter, major differ-
ences between the estimated and experimental RSI
values have been obtained, in some cases, values
differing by 10 points.
The Iscor model is based on the relationship
between CSR and a parameter F (Goscinski et al.,
1985; Goscinski and Patalsky, 1990):
CSR ¼ 2:56F � 15:52
where F is defined as a function of the maximum
vitrinite reflectance (Rmax), Gieseler maximum fluid-
M.A. Dıez et al. / International Journal of Coal Geology 50 (2002) 389–412400
ity in ddpm (MF), percentage of the inert content of
organic nature, and ash components, as follows:
F ¼ ½Rmax �MF�=½ðNa2Oþ K2OÞðCaOþMgO
þ Fe2O3Þ ðOrganic inertsÞ�
A modified basicity index (MBI) has been also
introduced by CANMET. The MBI is calculated from
coal ash chemistry and proximate analysis (Price et
al., 1988, 1992; Gransden et al., 1991):
MBI ¼ ½ð100AÞ=ð100� VMÞ� ½ðNa2Oþ K2O
þ CaOþMgOþ Fe2O3Þ=ðSiO2 þ Al2O3Þ�
where A and VM are the ash and volatile matter
contents in coal.
The MBI provides an estimation of the amount of
the basic components in the coke. A good relationship
between CSR and MBI was found, which can be
improved by considering petrographic data (mean
vitrinite reflectance) and dilatation parameters.
For 33 Cretaceous and 22 Carboniferous coals, a
correlation coefficient of 0.94 and a standard devia-
tion of 3.4 were obtained. When applied to the 33
Cretaceous coals and blends, the same correlation
coefficient was obtained, and the standard deviation
was 3.3. The model cannot be applied, however, to
oxidized (weathered) coals and it is restricted to the
coking conditions applied.
Recently, this prediction model has been modified
by BHP works in two ways: (1) by introducing the
coal dilatation temperature range as a new parameter
in the equation; and (2) by substituting the MBI by
(MBI)2. With these modifications, the CSR can be
predicted with a standard deviation of 2.72. However,
the authors indicated that caution should be taken
when applying the model to some of the coals tested
(McKenzie et al., 1998).
Based on the most significant correlation found
between CSR and the coal plastic range, (calculated as
the difference between the solidification temperature
and the softening temperature measured by Gieseler
plastometer), compared to those found for other
parameters such as maximum fluidity, total dilatation
and free-swelling index, a prediction model has been
developed at Inland Steel. The CSR prediction model,
first published in a brief paper (Valia, 1987) and later
reported in detail (Valia, 1989), introduced the range
of plasticity as a parameter reflecting rank and rheo-
logical properties of coal. The other term in the
multiparameter equation is the catalytic index (CI),
which takes account the combined effect of ash
chemistry and sulfur. The CI was defined as:
CI ¼ 9:64 alkali indexþ 14:04 sulphur content
The alkali index used is calculated as a product of
ash content and the weight percent ratio of the basic
(Fe2O3 + CaO + MgO + Na2O + K2O) and acidic
(SiO2 +Al2O3) components.
The equation used in the prediction model for
CSR, equally applied for single coals and blends, is
CSR ¼ 28:91þ 0:63PR� CI
where PR is the plastic range in jC; and CI is a
catalytic index (defined above).
To justify the introduction of the above terms in the
equation, the following considerations apply: (a) the
increase in plastic range optimizes the extent and size
of anisotropic carbon from mesophase which, in turn,
decreases the reactivity to carbon dioxide (Valia,
1989); (b) the increase in alkalis, iron, and sulfur
may have a double effect on CSR. On one side,
creating functional groups that affect fluidity and
inhibit growth of crystallites and on the other acting
as a catalyst of gasification by carbon dioxide (Marsh
and Walker, 1979).
The application of the Inland Steel prediction
model is valid for the range of coals investigated in
the study quoted: plastic range from 34 to 117.5 jC,catalytic index from 14.77 to 39.20, mean vitrinite
maximum reflectance from 0.65% to 1.65%, total
inerts from 3% to 30%, maximum fluidity from 2 to
>30000 ddpm, and the controlled conditions in the
pilot oven (Valia, 1989).
In an attempt to apply the model to coals with high
organic inert contents such as the Western Canadian
and some Australian coals, where it seems that these
organic inerts are not truly inerts, knowledge of
inertinite behavior must be considered.
The CSR prediction models described are aided by
the fact that CSR is additive. However, opposite views
on this matter have been reported. Some authors
M.A. Dıez et al. / International Journal of Coal Geology 50 (2002) 389–412 401
found that estimation of CSR by application of the
additivity rule is not that accurate (Chiu, 1982; Ber-
nard et al., 1986; Barsotti and Damiani, 1988; Ishi-
kawa et al., 1990), while others claimed that CSR is
an additive property (Caldeira and Da Silva, 1988;
Morishita et al., 1986; Valia, 1989).
The above prediction models are based exclusively
on different coal characteristics. Among the limita-
tions of these models, most are not valid when coal
was weathered (oxidized) during storage. Other pre-
diction models of coke strength, CRI, and CSR using
coke structure and properties (ash chemistry, porosity
parameters deduced from image analysis, optical
textural components) have been extensively reported,
as well as comparisons between quality of cokes
produced at pilot and industrial scales. The latter
constitute the third-generation of prediction models
that use statistical analyses of cokes produced in a
sole-heated oven, small pilot, and pilot coke ovens.
4. Coke production and demand
The blast furnace needs metallurgical coke and,
therefore, the demand and market for both coal and
coke will remain closely related to the steelmaking
industry. In 1999, the world equivalent crude steel
production accounted for 787 Mt with a hot metal
production of about 540 Mt (Terjung, 2000; Terjung
and Hermann, 2000; Wessiepe and Karsten, 2000).
Consequently, the hot metal to crude steel ratio was
approximately 700 kg t� 1 crude steel. The growth of
steel production is estimated for the next 15 years to be
between an optimistic 975 Mt and a pessimistic 840
Mt. Increases in production could be especially high in
the developing countries and could come from an
expansion in electric furnace processes and a growth
of hot metal production in existing blast furnaces
(Derycke and Bonte, 2000). However, although the
relative importance of electrical furnaces will increase
during the next decades, especially in emerging coun-
tries, and will influence coal/coke demand, the blast
furnace will continue to be the main process for crude
steel production in the near future.
Coke quantity is the largest of the charge materials
going into the blast furnace. In order to reduce costs
and diminish operational and environmental prob-
lems, coke has been substituted in part by other fuels
such as oil, granulated and pulverized coal (Cross,
1994), and more recently by plastic wastes (Janz and
Weiss, 1996; Imai, 1999; Asanuma et al., 2000; Ohji,
2000). Following the use of PCI technology, the ratio
coke/hot metal has changed from 1:1 (some 50 years
ago) to 250 kg of both coal and coke per ton of hot
Fig. 6. Evolution of coke production during the period 1990–1999.
M.A. Dıez et al. / International Journal of Coal Geology 50 (2002) 389–412402
metal. To achieve this PCI rate, especially high quality
coke is needed together with advanced technologies
both in coke production and blast furnace operation
(Lungen and Poos, 1996; Bertling, 1999; Terjung,
Demand for blast furnace coke in industrialized
countries will drop due to higher PCI rates. Data taken
from a world production review reported in the
journal, Cokemaking International (2000), shows that
coke production decreased in the early 1990s espe-
cially in Europe, North America, CIS, and Japan. This
decline was compensated by Chinese coke production
that has grown significantly from 43 Mt in 1980 to
139 Mt in 1997 (Fig. 6). From 1997, a decrease of
about 18 Mt was reported in Chinese coke production.
On a worldwide level, in 1997, there was a production
of 360 Mt coke, falling to about 324 Mt in 1999 (Fig.
7). Fig. 8 illustrates the global distribution of coke
production in 1999. Studies of the International Iron
and Steel Institute (IISI) (1997) predict a shortage of
coke by the year 2005, especially in Japan and USA
(Hofherr, 2000). However, the world demand for the
period 2000–2005 may be forecast at about 349 Mt of
coke. A decline in coke production capacity relates to
the age of installed cokemaking plants where huge
investments would be needed to built new coke plants
or renovate the old ones. The relative importance of
an international coke trade is not that high; in 1999, it
only accounted for about 5% of total coke production.
The usual situation is that the coke is produced and
consumed locally within integrated metallurgical
works and steel mills. China during the last few years
has become the biggest coke producer and exporter in
the world, exporting to the USA, Brazil, and European
countries. One of the problems of the use of imported
coke is the lack of homogeneity and many consumers
only use it as an admixing component.
Due to the double use of coal in the ironmaking
industry, the situation of coal is quite different to that
of the coke. On one side, amounts of coal for use in
the blast furnace operating with PCI are expected to
increase in the future (Trickett, 1999). No special
Fig. 7. Worldwide coke production for the period 1990–1999.
Fig. 8. Worldwide distribution of coke production on the basis of 324.4 Mt for 1999. E: estimated.
M.A. Dıez et al. / International Journal of Coal Geology 50 (2002) 389–412 403
requirements are needed for such coals and they are
readily available without problems. In general, carbon
and hydrogen contents are key parameters for PCI as
well as the absence of coking ability and a coal
chemistry quite similar to that required for coking
coals. On the other hand, coking coals are needed to
produce metallurgical coke with very strict quality
specifications. Generally speaking, coke is produced
with a yield of 75 wt.%, so to produce 340 Mt within
the 250 coking plants of the world, about 450 Mt of
coking coal are needed. Excellent coking coals are
produced in Australia, Canada, USA, and Poland.
About 60% of coal mined is used in the country of
origin and the rest is exported to Japan and Europe
(Bertling, 1999). No shortage is expected in the next
years, specially taking into account the high produc-
tivity of Australia and Canada. For the future, growth
in consumption is only expected in countries such as
China, Korea and Taiwan.
5. Coking processes of the future
On the industrial scale, present trends in coke
manufacture are to use classical multi-chamber bat-
teries with horizontal slot-like ovens and circular open-
ings in the top for charging coal into the oven,
removable doors through which the coke is discharged,
laterally arranged heating walls in the upper oven
section, regenerator heat exchangers in the lower sec-
tion, and a substructure that includes waste heat ducts.
In conventional carbonisations, about 15 to 30 t of
coal blend, crushed to 80% < 3 mm particle size, is
charged into the hot oven by gravity. The ovens are
heated to a temperature of about 1200–1300 jCthrough the side-walls, which are kept at as uniform
temperature as is possible. As the coal is gradually
heated from both walls to the centre, a temperature
gradient exists which decreases as the carbonization
proceeds. This means that in the early stages of the
carbonization process, the coal layer in contact with a
side-wall is rapidly heated, while the centre of the coal
charge remains at a relatively low temperature. When
the temperature of the centre is 900 to 1000 jC, andafter a period of soaking, the coking cycle is completed.
A total period of 18–20 h is required for blast furnace
coke production, the time depending on the oven
dimensions. In the 1970, dimensions of by-product or
slot-type coke ovens were commonly of 12–16 m
length, 4–8 m height, and 400–450 mm width to
ensure a good heat transmission from the oven wall
to the centre. Very recent coke ovens in Germany have
dimensions that exceed the recognized limits in all the
three dimensions. Tables 3 and 4 summarize the state of
the art in 1970s and 1980s, respectively, for a coke
capacity of 2 Mt year� 1 (Nashan, 1987). The gradual
enlargement in chamber dimensions to near 8 m height,
16–18 m length, and 550–610 mm wide and in oven
volume 70–79 m3 reduces the number of ovens needed
for the same production. Advantages claimed for these
larger capacity ovens are: (a) low specific investment
costs; (b) low heat losses; (c) small space requirements;
and (d) improvements in environmental protection due
to the decreased number of oven chamber openings as
well as a shorter time period for charging. The Kaiser-
tuhl III coking plant in Germany, with two batteries of
60 ovens each, represents the most advanced state of
the development of the multi-chamber system incor-
porating the know-how and experience of more than
100 years. With this coking plant, inaugurated in
December 1992, producing 2 Mt of coke per year, the
development of multi-chamber systems reached the
highest technological level in the last 100 years with
successful results (Ameling et al., 1999).
State of the art of coking plants with a capacity of 2 Mt coke per
year in the 1970s (Nashan, 1987)
Coking plant (size)
Small Medium Large
Height (m) 4.50 6.00 7.65
Length (m) 11.70 14.20 16.40
Width (mm) 450 450 435
Useful volume (m3) 22.1 36.4 52.2
per oven (t)
22.1 36.4 52.2
Number of ovens 322 187 123
Total oven openings 2898 1496 984
Length of sealing
10.5 6.9 5.1
Number of pushed
ovens per day
430 257 171
Total opening cycles
3870 2056 1368
Length of sealing faces
to be cleaned
(km day� 1)
14.0 9.5 7.2
M.A. Dıez et al. / International Journal of Coal Geology 50 (2002) 389–412404
Noting that future steel production will still be
associated with conventional ironmaking via coke
oven/blast furnace, the development of new coking
systems is further accelerated by problems associated
with the limitations reached in multi-chamber system;
by current expenditures on pollution control being
25% and 30% of the specific investment and operat-
ing costs, respectively (Ameling et al., 1999); work
place conditions to comply with strict environmental
requirements; the maximum permissible wall pressure
in multi-chamber systems which limits the design of
coal blends; and finally the extreme age of existing
Concerning the age of coke oven batteries, they
have a possible economical life of 20 to 30 years and
an environmental life of 10 to 20 years. This means
that an average service life is of about 25 years. The
battery can operate for another 15 years, reaching a
technical life of 30 to 40 years, but only with high cost
maintenance. Because of the high investment cost of a
new coke plant, the option of the extension of the
lifetime is common practice. Improvements and
developments in repair technology in the last decades
have extended the life of coke batteries and provided
optimum environmental behaviour. However, at
present more than 50% of the installed capacity for
coke manufacture is over 25 years of age (Nashan et
al., 2000a). But it has to be stressed that high quality
coke will still be required by blast furnaces in suffi-
cient quantity to ensure future iron and steel produc-
tion. As a consequence, even with the use of PCI in
blast furnaces, coke demand, in the short and medium
term, cannot be met safely. Coke supplies from tradi-
tional exporting countries like China will also decline
due to the closure of primitive and out-dated facilities.
It is not surprising, then, that at the very beginning of
the 21st century, several papers present opinions on
cokemaking technology for the 21st century. The
present status in individual countries and how to meet
future demand have been analysed in the two volumes
of the journal Cokemaking International (Blanco,
2000; Deshpande, 2000; Kiessling and Sundholm,
2000; Kovalev et al., 2000; Liu et al., 2000; Nashan
et al., 2000b; Pensa, 2000; Rudyka, 2000; Sciazko,
On the basis of the above considerations, a stage
may be reached at which coke producers will make
decisions on the modernization and repairing of
existing coking plants, on the construction of new
batteries, or to access the restricted coke market.
Starting at the end of the 20th century, the develop-
ment of 21st century technology appears to be the
reaction towards increasing future supplies. The new
cokemaking technologies address the development of
an environmentally friendly technology with high
productivity and a more flexible utilization of weakly
and non-coking coals in the blends carbonized.
Different approaches at different stages of develop-
ment consider two-product technologies, non-recov-
ery ovens, and single chamber system (SCS). They
offer an interesting alternative to conventional coke
ovens where the demand is only for coke and not for
gas and other by-products such as benzol, tar, and
ammonia. Other technologies being developed keep
the conventional multi-chamber system with by-prod-
ucts recovery from coke-oven gas and waste water in
additional installations, but introduce coal pre-treat-
ment and coke post-treatment in special design instal-
lations (SCOPE 21).
5.1. The non-recovery coke oven
This new approach in cokemaking technology
resembles the early beehive ovens that carbonized
coal in horizontal layers, being of simple design,
State of the art of coking plants with a capacity of 2 Mt coke per
year in the 1980s (Nashan, 1987)
Huckingen Prosper Kaiserstuhl III
Height (m) 7.85 7.10 7.63
Length (m) 17.20 15.90 18.00
Width (mm) 550 590 610
Useful volume (m3) 70.0 62.3 78.9
per oven (t)
43.0 39.8 48.7
Number of ovens 120 142 120
Total oven openings 1080 1278 1080
Length of sealing
6.0 6.2 5.5
Number of pushed
ovens per day
128 138 115
Total opening cycles
1152 1242 1035
Length of sealing faces
to be cleaned
(km day� 1)
5.6 6.0 5.3
M.A. Dıez et al. / International Journal of Coal Geology 50 (2002) 389–412 405
and operation. In the Jewell–Thompson non-recovery
ovens, the volatile products produced during coal
carbonization are not recovered. The evolved gas,
including benzol and tar, is burnt directly in the oven
space above the coal, thus generating the heat needed
for the process. The mixture of crude and waste gases
is led through vertical ducts in the side-walls to the
heating flue system under the oven sole. There the
combustion is completed by the staged supply of air
so that the coal layer is evenly heated from the top and
bottom. The hot waste gas is cooled in waste heat
boilers to raise steam, which can either be fed into the
steam grid or used for generating electricity. As an
estimation, about 75–95 MW electric power can be
generated for a coke production of 1 Mt year� 1,
depending on the volatile matter content of the coal
and the composition of the coal blend charged. The
exploitation of the waste gas is a major improvement
over old beehive ovens of the 19th century (Ellis and
Schuett, 1999; Walker, 1999; Westbrook and Schuett,
2000). The dimensions of the non-recovery ovens are
about 13.5 m long, 4.6 m wide, and 2.4 m high at the
crown of the arch, the thick coal layer being of
approximately 1 m. The coal charged into the oven
accounts weighs about 36 to 41.5 t (Ellis and Schuett,
1999) with a coking time of 48 h. Depending of the
volatile matter of the blend carbonized, the charge
weight, coke yield, and coking time will vary.
In USA, the Sun Coke non-recovery or heat
recovery technology was first developed at the Jewell
coke plant in Vansant, Virginia, producing 635,000 t
of coke. Recently, the first high capacity plant (Indi-
ana Harbor Coke facility) with four batteries of 67
heat-recovery ovens each, representing the advanced
developed of the Jewell–Thompson non-recovery
ovens, has been put into operation at Inland Steel
Chicago. It was designed to produce about 1.2 Mt of
screened coke per year and 94 MW of power gen-
eration. Fig. 9 displays a schematic diagram of this
plant. Technical details are reported after 1 year (Ellis
and Schuett, 1999) and 2 years (Westbrook and
Schuett, 2000) of operation. This technology has
emerged as a virtually clean technology. As the ovens
operate under suction, no emissions during the coking
process and wastes derived from by-products facilities
On the other hand, lateral coking pressure of a coal
blend is much less important than in conventional coke
ovens. This means that the use of coals or coal blends,
which develop a higher coking pressure, is not a
limitation and they can be carbonized without any
danger for the non-recovery ovens. From 1998, differ-
ent coal blends containing from three to six coals have
been used at Indiana Harbor facility. Two types of coal
blends were used, a relatively high-volatile blend of
28.6 wt.% dry basis and a low-volatile blend of 24.5
wt.% dry basis. As regards coke quality, CSR ranged
from 67% to 72% and stability from 60% to 64%.
With this new technology, prediction models have
been also developed for such coke properties, stability
Fig. 9. Schematic diagram of the non-recovery oven system.
M.A. Dıez et al. / International Journal of Coal Geology 50 (2002) 389–412406
and CSR. The models are based on a so-called ‘‘fish-
bone’’ diagram, which includes the factors affecting
coke quality grouped in different categories and sub-
5.2. Single chamber system (SCS)
In September 1987, during the first International
Cokemaking Congress held in Essen, Germany, the
single chamber or coking reactor system with two
basic proposals for the design of the so-called Jumbo
Coking Reactor—JCR (with underneath- and side-ar-
ranged regenerators) was presented (Nashan, 1987).
To explore the possibilities of the JCR as a new
cokemaking technology for the 21st Century, the Eu-
ropean Community accepted a European project in
1990. For the EUREKA project development, the
European Cokemaking Technology Centre (ECTC)
was created with the leadership of the German coking
industry and 11 companies representing seven Euro-
The SCS combines coal preheating to temperatures
of 180 to 200 jC with dry coke quenching. It
abandons the multi-chamber system in favour of a
single and independent reactor and avoids the recov-
ery of by-products from coke-oven gas, producing
only two products—coke and hydrogen gas-rich prod-
uct (Nashan, 1987, 1990, 1992). The recovered crude
gas can be used as traditional energy source in steel
mills, for steam and electric power generation, or as a
reducing gas in iron ore reduction process (Ameling et
al., 1999; Nashan et al., 2000c). Fig. 10 shows the
concept of the SCS technology. In the 1990s, different
stages of the construction and progress of the demon-
stration plant built in Prosper-Germany and results
obtained were reported (Bertling and Rohde, 1994,
1995, 1996, 1997; Ameling et al., 1999; Baer, 2000;
Nashan et al., 2000a, 2000c).
The single coking reactor built in 1992 and oper-
ated by ECTC, having dimensions of 10 m high, 10 m
long, and 0.85 m wide, was charged with preheated
coal and produce about 50 t coke per charging cycle.
During the trial period, evaluations of coking con-
ditions (bulk density, coking rate and time, and final
coke temperature), emission control, coal blend char-
acteristics (volatile matter content between 25 and 31
wt.%), and coke quality in terms of CRI and CSR
parameters were made. As regards to coking pressure,
the SCS is able to withstand high generated coking
pressures due to the rigidity of the heating wall (>300
vs. 100 mbar in conventional multi-chamber system)
(Nashan et al., 2000a, 2000c). Using high-volatile
coals, the coke obtained was less porous as a result
of the preheated coal charges, less reactive, and highly
resistant to mechanical stresses (Bertling and Rohde,
1994). For comparison purposes with the SCS tech-
nology, the coal blends were also carbonized in multi-
chamber system and the coke quality evaluated.
Results using single coals, two- and four-component
blends with amounts ranging from 30% to 80% of
Fig. 10. Schematic diagram of the single chamber system (SCS).
M.A. Dıez et al. / International Journal of Coal Geology 50 (2002) 389–412 407
poor-coking coals and 10% to 50% of non-coking
coals (Bertling and Rohde, 1996) and multi-compo-
nent blends, at the final stage of demonstration,
showed the flexibility of the SCS in the use of a great
proportion of cheaper poor- and non-coking coals in
the blends and the improvement in coke quality, in
particular the CSR values (Nashan et al., 2000a).
At present, the SCS, initially known as the Jumbo
Coking Reactor, is proposed to be ready for an
industrial scale application. A new stimulus from the
cokemaking industry, at the beginning of the 21st
century, is needed.
5.3. SCOPE 21
As an alternative to conventional coking process,
the Japan Iron and Steel Federation is promoting the
development of a new system under a project called
the ‘‘Super Coke Oven for Productivity and Environ-
ment enhancement in the 21st century’’ (SCOPE 21).
It is an 8-year project started in 1994 (Nishioka, 1996;
Kubo, 1996; Sasaki et al., 1998; Nakashima, 1999;
Taketomi et al., 2000).
In this new coking design, the conventional coking
process is divided into three separated stages: the pre-
treatment of coal blend, the medium-temperature
coking process, and the upgrading of coke followed
by coke dry quenching. The initial step consists of the
separation of fine coal particles < 0.3 mm and coarse
coal particles >0.3 mm and the separated rapid heating
to near to the temperature of thermal decomposition of
coal (350–400 jC). The fine coal is agglomerated by
hot briquetting and charged into a conventional coke
oven together with the preheated coarse coal. The next
stage is a coking process at a much lower temperature
(750–850 jC) than in conventional process. The coke
is finally discharged and subjected to a further heat
treatment up to 1000 jC in the upper part of the CDQ
facility. Fig. 11 shows a schematic diagram of the
A bench scale test plant with 0.6 t h� 1 coal
processing capacity was built at NSC Nagoya works.
Test runs investigated the dry classification of coal,
with rapid heating and compaction of fine coal. The
results revealed that the combination of high bulk
density, rapid heating and carbonization gave an
acceptable coke quality even when using up to 50%
poor- or non-coking coals. After considering the
benefits of the new coking design in a blench scale,
a pilot plant test is planned to be performed in 2001.
5.4. Calderon coking reactor
Another cokemaking approach in development is
the Calderon Coking Reactor which is based on
continuous coking of coal in a heated tubular reactor.
The continuous process is designed as a two-step
process, including carbonization at low temperature
followed by calcination of the coke in a separate
device with complementary hot gas cleanup system.
In 1997, Bethlehem and US Steel joined with Cal-
deron Energy to further develop the process and to
check coal blends for the pilot scale plant (Strauss,
1999). The construction of a full size reactor is
Fig. 11. Schematic diagram of the SCOPE21 cokemaking system.
M.A. Dıez et al. / International Journal of Coal Geology 50 (2002) 389–412408
underway and it is planned to test the coke in a
commercial blast furnace.
At the very beginning of the 21st century, coal will
continue to be a dual source in blast furnace technol-
ogy with pulverized coal injected at the tuyeres and
coke as a permeable support. Extensive R&D in coal
blending and coke quality will be needed to meet the
blast furnace requirements. With a short- and medium-
time horizon, a new impulse is expected for clean and
cost-effective cokemaking technologies at the actual
stage of pilot scale trials and those at a more advanced
state together with improvements in conventional
The authors are grateful to Prof. Harry Marsh of
Newcastle upon Tyne (UK) for his helpful comments
during the preparation of this review.
Alvarez, R., Dıez, M.A., 2000. Chemistry of production of metal-
lurgical coke. In: Marsh, H., Rodrıguez-Reinoso, F. (Eds.), Sci-
ences of Carbon Materials, Chap. 18. Secretariado de Publica-
ciones, The University of Alicante, Spain, pp. 595–635.
Ameling, D., Baer, H., Bertling, H., Lungen, H.B., 1999. Cokemak-
ing technology 2000. State-of-the-art and new structures. Coke-
mak. Int. 11 (1), 32–39 (also in: Technical Exchange Session.
Int. Iron and Steel Institute (IISI), Committee on Technol-
ogy, Brussels, 1999, pp. 30–45).
Ammosov, I.I., Eremin, I.V., Sukhenko, S.F., Oshurkova, L.S.,
1957. Calculation of coking changes on basis of petrographic
characteristics of coals. Coke Chem. U.S.S.R. 2, 9–12.
Asanuma, M., Ariyama, T., Sato, M., Murai, R., Nonaka, T., Oko-
chi, I., Tsukiji, H., Nemoto, K., 2000. Development of waste
plastics injection process in blast furnace. ISIJ Int. 40, 244–251.
Baer, H., 2000. Cokemaking with the single chamber coking sys-
tem. Proc. 4th European Coke and Ironmaking Cong., ATS-RM,
Paris, vol. 2, pp. 659–663.
Barsotti, A., Damiani, R., 1988. Coal properties evaluation and
blending philosophy at Italsider as mean for predetermining
coke characteristics according blast furnace requirements. Proc.
47th Ironmaking Conf., ISS-AIME, pp. 163–171.
Barriocanal, C., Hanson, S., Patrick, J.W., Walker, A., 1994. The
characterization of interfaces between textural components in
metallurgical cokes. Fuel 73, 1842–1847.
Barriocanal, C., Alvarez, R., Canga, C.S., Dıez, M.A., 1998. On the
possibility of using coking plant waste materials as additives for
coke production. Energy Fuels 12, 981–989.
Benedict, L.G., Thompson, R.R., 1976. Selection of coals and coal
mixes to avoid excessive coking pressure. Proc. 35th Ironmak-
ing Conf., ISS-AIME, pp. 276–286.
Benedict, L.G., Thompson, R.R., Wenger, R.O., 1968a. Relation-
ship between coal petrographic composition and coke stability.
Blast Furn. Steel Plant 56 (3), 217–224.
Benedict, L.G., Thompson, R.R., Shigo, J., Aikinan, R., 1968b.
Pseudovitrinite in Appalachian coking coals. Fuel 47, 125–143.
Bernard, A., Duchene, J.M., Isler, D., 1985. Etude de la gazeifica-
tion du coke. Rev. Met. CIT 82, 849–860.
Bernard, A., Duchene, J.M., Vogt, D., Jeulin, D., Steiler, J.M.,
Bourrat, X., Rouzaud, J.N., 1986. Effect of rank and of inter-
actions of coals on experimental coke properties. Proc. 45th
Ironmaking Conf., ISS-AIME, pp. 211–219.
Bertling, H., 1999. Coal and coke for blast furnace. ISIJ Int. 39 (7),
Bertling, H., Rohde, W., 1994. Jumbo Coking Reactor. First opera-
tional experience with a new cokemaking technology. Cokemak.
Int. 6 (1), 8–11.
Bertling, H., Rohde, W., 1995. Jumbo Coking Reactor. Progress
report. Cokemak. Int. 7 (2), 20–25.
Bertling, H., Rohde, W., 1996. Jumbo Coking Reactor (JCR) and
two product coking process. Proc. 3rd European Cokemaking
Cong., CRM-VDEh, Gent, Belgium, pp. 273–278.
Bertling, H., Rohde, W., 1997. Coke quality improvements by SCS-
Technology. Cokemak. Int. 9 (1), 31–34.
Blanco, R., 2000. The coal and coke industries in Colombia.
Cokemak. Int. 12 (2), 56–57.
Brown, H.R., Taylor, G.H., Cook, A.C., 1964. Prediction of coke
strength from the rank and petrographic composition of Austral-
ian coals. Fuel 43, 43–54.
Bustin, R.M., Cameron, A.R., Grieve, D.A., Kalkreuth, W.D., 1985.
Coal petrology. Its principles, methods and applications, 2nd
revised ed. Geological Assoc. of Canada, Short Course Notes,
Victoria, British Columbia, vol. 3, pp. 167–203.
Caldeira, J.S., Da Silva, P.H.L., 1988. Microscopy as a means to
assess coke mechanism and behaviour under reactive condi-
tions. Proc. 47th Ironmaking Conf., ISS-AIME, pp. 357–360.
Carr, A.J., Jorgensen, J.G., 1975. An estimate of the effective re-
active/inert ratio of semifusinite in Western Canadian coals.
CANMET Rep. 75-141, 12 pp. (ref. taken from Gransden, J.F.
et al., 1991).
Chiu, Y.F., 1982. Study of coke petrography and factors affecting
coke reactivity. Ironmak. Steelmak. 9 (5), 193–199.
Cokemaking International, 2000. World production review. Coke-
mak. Int. 12 (2), 72–78.
Colleta, A., Barnaba, P., Federico, G., Masella, D.C., 1990. Influ-
ence of coal properties on high coke quality for blast furnace.
Proc. 49th Ironmaking Conf., ISS-AIME, pp. 243–252.
Cross, W.B., 1994. The future and the European steel industry and
its demand for coal. The Coke Oven Managers’ Association
(COMA) Year-Book, Mexborough, pp. 97–108.
Derycke, J., Bonte, L., 2000. Ironmaking perspectives for the early
21st Century. Proc. 4th European Coke and Ironmaking Cong.,
ATS-RM, Paris, vol. 2, pp. 693–702.
Deshpande, D.P., 2000. Cokemaking technology in India. Coke-
mak. Int. 12 (2), 60–62.
Dıez, M.A., Alvarez, R., Sirgado, M., Marsh, H., 1991. Preheating
M.A. Dıez et al. / International Journal of Coal Geology 50 (2002) 389–412 409
techniques to manufacture metallurgical coke. ISIJ Int. 31,
Dutcher, L.A.F., Crelling, J.C., 2000. History of applied coal pet-
rology in the United States: I. Early history of the application
of coal petrology in the steel industry. Int. J. Coal Geol. 42,
Edwards, D.G. (Ed.), 1991. The strength of coke after partial gas-
ification. BCRA Quarterly, Chesterfield, UK, No. 30, pp. 37–
Ellis, A.R., Schuett, J., 1999. Heat recovery cokemaking at Indiana
Harbor coke company—one year of operation. Cokemak. Int. 11
Falcon, R.M.S., Snyman, C.P., 1986. An introduction to Coal Pet-
rography: Atlas of Petrographic Constituents in the Bituminous
Coals of Southern Africa. The Geology Society of South Africa,
Johannesburg, 27 pp.
Fujita, H., Hijiriyama, M., Nishida, S., 1983. Gasification reactivities
of optical textures of metallurgical cokes. Fuel 62, 875–879.
Gibson, J., 1972. Dilatometry and the prediction of coke quality.
The Coke Oven Managers’ Association (COMA) Year-Book,
Mexborough, pp. 182–205.
Gibson, J., Gregory, D.H., 1978. Selection of coals and blend prep-
aration for optimum coke quality. The Coke Oven Managers’
Association (COMA) Year-Book, Mexborough, pp. 159–182.
Goscinski, J.S., Patalsky, R., 1990. CSR control. A coal producers
point of view. Proc. 49th Ironmaking Conf., ISS-AIME, pp.
Goscinski, J.S., Gray, R.J., Robinson, J.W., 1985. A review of
American coal quality and its effect on coke reactivity and after
reaction strength of cokes. J. Coal Qual. 4 (2), 21–29.
Gransden, J.F., Jorgensen, J.G., Manery, N., Price, J.T., Ramey,
N.J., 1991. Applications of microscopy to cokemaking. Int. J.
Coal Geol. 19, 77–107.
Großpietsch, K.H., Lungen, H.B., Dauwels, G., Ferstl, A., Karja-
lahti, T., Negro, P., van der Velden, B., Willmers, R., 2000. Coke
quality requirements by European blast furnace operators on the
turn of the millennium. Proc. 4th European Coke and Ironmak-
ing Cong., ATS-RM, Paris, vol. 1, pp. 2–11.
Hara, Y., Mikuni, O., Yamamoto, H., Yamanaka, Y., 1980. The
assessment of coke quality with particular emphasis on sampling
technique. In: Lu, W.K. (Ed.), McMaster Symposium on Iron
and Steelmaking. McMaster Symposium, McMaster University,
vol. 8, pp. 4.1–4.38.
Harrison, J.A., Jackman, H.W., Simon, J.A., 1964. Predicting coke
stability from petrographic analysis of Illinois coals. Illinois
State Geological Survey, Circular, vol. 366, 20 pp.
Hatano, M., Miyazaki, T., Iwanaga, Y., 1990. Analysis of blast
furnace operation based on the mathematical model for evalua-
tion of coke properties. Coke Reactivity and its Effects on Blast
Furnace Operation. The Iron and Steel Society, pp. 21–34.
Hofherr, K., 2000. State of the art in cokemaking and future devel-
opment. Proc. 4th European Coke and Ironmaking Cong., ATS-
RM, Paris, vol. 2, pp. 686–692.
Horrocks, K.R.S., Cunningham, R.B., Ellison, J.F., Nightingale,
R.J., 2000. Coke quality at BHP Steel Port Kembla. Proc. 4th
European Coke and Ironmaking Cong., ATS-RM, Paris, vol. 1,
Hyslop, W., 1981. Carbon solution and coke quality. The Coke
Oven Managers’ Association (COMA) Year-Book, Mexbor-
ough, pp. 131–182.
Imai, T., 1999. Production and technology of iron and steel in Japan
during 1998. ISIJ Int. 39, 509–523.
International Iron and Steel Institute (IISI), 1997. Coke and
its Alternatives. Committee on Raw Materials, Brussels,
Ishikawa, I., Case, M., Abe, Y., Ono, K., Sugata, M., Nishi, T.,
1990. Influence of post-reaction strength of coke on blast fur-
nace operation. Coke Reactivity and its Effects on Blast Furnace
Operation. The Iron and Steel Society, pp. 37–48.
Janz, J., Weiss, W., 1996. Injection of waste plastics into the blast
furnace of Stahlwerke Bremen. Proc. 3rd European Cokemaking
Cong., CRM-VDEh, Gent, Belgium, pp. 114–119.
Kaegi, D.D., Valia, H.S., Harrison, Ch.H., 1988. Maceral behaviour
and coal carbonisation. Proc. 47th Ironmaking Conf., ISS-
AIME, pp. 339–349.
Kiessling, F., Sundholm, J., 2000. Cokemaking in the United States.
Cokemak. Int. 12 (2), 67–68.
Kovalev, E.T., Sklyar, M.G., Shulga, I.V., Starovoit, A.G., 2000.
Main trends of development of cokemaking facilities in Uk-
raine. The view and assessment of UKhIN and UKRKOKS.
Cokemak. Int. 12 (2), 64–65.
Kubo, S., 1996. Recent trends in the Japanese steel and coke in-
dustries and the concepts of a new cokemaking process. Proc.
3rd European Cokemaking Cong., CRM-VDEh, Gent, Belgium,
Leeder, W.R., Price, J.T., Gransden, J.F., 1997. Western Canadian
coals. Thermal and rheology and coking quality. Proc. 56th
Ironmaking Conf., ISS-AIME, pp. 37–44.
Leonard, D.C., Bonte, L., Dufour, A., Ferstl, A., Raipala, K.,
Scmole, P., Schoone, P., Verduras, J.L., Willmers, R.R., 1996.
Coke quality requirements of European blast furnace engineers
(joint EBFC-Paper). Proc. 3rd European Cokemaking Cong.,
CRM-VDEh, Gent, Belgium, pp. 1–10 (also in: The Coke
Oven Managers’ Association (COMA) Year-Book, Rother-
ham, 1997, pp. 279–303).
Liu, H., Cai, Ch., Zheng, W., 2000. China’s coking industry step-
ping into the new century. Cokemak. Int. 12 (1), 48–53.
Loison, R., Foch, P., Boyer, A., 1989. Coke. Quality and Produc-
tion. Butterworth, London, pp. 178–189.
Lungen, H.B., Poos, A., 1996. Injection of coal into the blast fur-
nace. Cokemak. Int. 9 (2), 14–31.
Mackowsky, M.Th., Simonis, W., 1969. Die Keenzeichnung von
Kokskohlen fur die mathematische Beschreibung der Hochtem-
peraturverkokung in Horizontalkammerofen bei Schuttebetrieb
durch Ergebnisse mikroskopischer Analysen. Gulckauf-For-
schungsheft 30, 25–37.
Marsh, H., 1982. Metallurgical coke: formation, structure and prop-
erties. Proc. 41st Ironmaking Conf., ISS-AIME, pp. 2–11.
Marsh, H., 1992. The coke making process. Proc. 51st Ironmaking
Conf., ISS-AIME, pp. 569–580.
Marsh, H., Clarke, D.E., 1986. Mechanisms of formation of struc-
ture within metallurgical coke and its effects on coke properties.
Erdol Kohle Erdgas Petrochem. 39, 113–122.
Marsh, H., Walker Jr., P.L., 1979. The effects of impregnation of
M.A. Dıez et al. / International Journal of Coal Geology 50 (2002) 389–412410
coal by alkali salts upon carbonisation properties. Fuel Process.
Technol. 2, 61–75.
McKenzie, F., Hockings, K., Livingstone, P., 1998. Modelling of
coal blending to predict coke quality. Proc. AIE 8th Australian
Coal Science Conf., Sydney, pp. 101–106.
Menendez, J.A., Pis, J.J., Alvarez, R., Barriocanal, C., Fuente, E.,
Dıez, M.A., 1996. Characterization of petroleum coke as an
additive in metallurgical cokemaking. Modification of thermo-
plastic properties of coal. Energy Fuels 10, 1262–1268.
Menendez, J.A., Pis, J.J., Alvarez, R., Barriocanal, C., Canga, C.S.,
Dıez, M.A., 1997. Characterization of petroleum coke as an
additive in metallurgical cokemaking. Influence on metallurgical
coke quality. Energy Fuels 11, 379–384.
Menendez, J.A., Alvarez, R., Pis, J.J., 1999. Determination of met-
allurgical coke reactivity at INCAR: NSC and ECE-INCAR
reactivity tests. Ironmak. Steelmak. 26, 117–121.
Miura, Y., 1978. The science of cokemaking technology and its
development in Japan. The Coke Oven Managers’ Association
(COMA) Year-Book, Mexborough, pp. 292–311.
Miyazu, T., 1974. The evaluation and design of blends using many
kinds of coals for cokemaking. Int. Iron Steel Cong., Dussel-
dorf, Pap. 22.214.171.124.
Morishita, N., Tsukada, K., Suzuki, N., Nemoto, K., 1986. Devel-
opment of automatic coal/coke microscopic analyzer and its
application to cokemaking. Proc. 45th Ironmaking Conf., ISS-
AIME, pp. 203–209.
Moses, R., 1976. Use of Petrographic Analysis for the Prediction of
Coke Stability Report Bituminous Coal Research, Monroeville,
PA, 19 pp.
Munnix, R., 1984. Coke strength prediction based on coal petrog-
raphy and fluidity measurements. Proc. 43rd Ironmaking Conf.,
ISS-AIME, pp. 19–27.
Nakamura, N., Togino, Y., Tateoka, T., 1977. Behaviour of coke in
large blast furnace. Coal, Coke and Blast Furnace. The Metals
Society, London, pp. 1–18.
Nakashima, Y., 1999. Scope 21 cokemaking process. Technical
Exchange Session. Int. Iron and Steel Institute (IISI), Committee
on Technology, Brussels, pp. 16–29.
Nandi, B.N., Montgomery, D.S., 1975. Nature and thermal behav-
iour of semi-fusinite in Cretaceous coal from Western Canada.
Fuel 54, 193–196.
Nashan, G., 1987. The production of blast-furnace coke can be se-
cured in the long term ecologically beneficial and cost-efficiently.
On the way to a new coking system. Preprints 1st Int. Cokema-
king Congr., vol. 1, A2. Verlag Gluckauk, Essen, 51 pp.
Nashan, G., 1990. European development centre for cokemaking
technology—tasks and targets. Cokemak. Int. 2 (2), 19–29.
Nashan, G., 1992. Economic fundaments for new cokemaking sys-
tem and a new process structure of a coke plant—Jumbo Coking
Reactor. Proc. 51st Ironmaking Conf., ISS-AIME, pp. 349–358.
Nashan, G., Rohde, W., Wessiepe, K., Winzer, G., 2000a. Modular
and 2-product technology. The cokemaking process for the fu-
ture. Proc. 4th European Coke and Ironmaking Cong., ATS-RM,
Paris, vol. 2, pp. 646–653.
Nashan, G., Rohde, W., Wessiepe, K., 2000b. Long term perspec-
tives for cokemaking technology from individual country’s
view. Cokemak. Int. 12 (1), 44–47.
Nashan, G., Rohde, W., Wessiepe, K., 2000c. Some figures and
facts on the present status and new proposals for a future-ori-
ented cokemaking technology. Cokemak. Int. 12 (2), 50–55.
Negro, P., Steiler, J.M., Beppler, E., Jahusen, U., Bennington, C.R.,
Willmers, R.R., 1996. Assessment of coke degradation in the
blast furnace from tuyeres probing investigations. Proc. 3rd
European Ironmaking Cong., CRM-VDEh, Gent, Belgium, pp.
20–27 (also in: The Coke Oven Managers’ Association
(COMA) Year-Book, Rotherham, UK, 1997, pp. 256–278).
Nishioka, K., 1996. Challenge for innovative cokemaking process
in Japan. Proc. 3rd European Cokemaking Cong., CRM-VDEh,
Gent, Belgium, pp. 285–290.
Nishioka, K., 2000. History and future of the Japanese coke-
making technology. J. Jpn. Inst. Energy 79 (876), 284–298
O’Donnell, E.M., Poveromo, J.J., 2000. Coke quality requirements
from a North American perspective. Proc. 4th European Coke
and Ironmaking Cong., ATS-RM, Paris, vol. 1, pp. 12–19.
Oguri, K., Kitahara, A., Hijiriyama, M., Nishida, S., Aketa, K.,
1987. Evaluation of coking coal. Preprints 1st Int. Cokemaking
Cong., vol. 1, E1. Verlag Gluckauk, Essen, 12 pp.
Ohji, M., 2000. Production and technology of iron and steel in
Japan during 1999. ISIJ Int. 40, 529–543.
Okuyama, Y., Miyazu, T., Sugimura, H., Kumagai, M., 1970. Pre-
diction of the coking property of coal by microscopic analysis. J.
Fuel Soc. Jpn. 49 (522), 736–743.
Patrick, J.W., Walker, A., 1995. Porosity and strength of carbon
materials. In: Patrick, J.W. (Ed.), Porosity in Carbons: Charac-
terization and Applications, Chap. 7. Edward Arnold, UK, pp.
Patrick, J.W., Wilkinson, H.C., 1978. Analysis of metallurgical
cokes. In: Karr Jr., C. (Ed.), Analytical Methods for Coal and
Coal Products, vol. II. Academic Press, NewYork, pp. 339–370.
Patrick, J.W., Wilkinson, H.C., 1981. Coke reactivity. The Coke
Oven Managers’ Association (COMA) Year-Book, Mexbor-
ough, UK, pp. 191–220.
Pearson, D.E., Price, J.T., 1985. Reactivity of inertinite (coal-typ-
ing) of Western Canadian coking coal. Proc. Int. Conf. on Coal
Science. Pergamon Press, Sydney, pp. 907–908.
Pensa, R., 2000. Future perspectives for cokemaking technology:
current situation in Italy. Cokemak. Int. 12 (2), 58–59.
Poos, A., 1987. Constitution and monitoring of coking coal blends.
The Coke Oven Managers’ Association (COMA) Year-Book,
Mexborough, UK, pp. 223–253.
Poveromo, J.J., 1996. Operational considerations for high-level
blast furnace fuel injection. Proc. 55th Ironmaking Conf., ISS-
AIME, pp. 79–92.
Price, J.T., Gransden, J.F., Khan, M.A., 1988. Effect of the proper-
ties of Western Canadian coal on their coking behaviour. Proc.
47th Ironmaking Conference, ISS-AIME, Toronto, pp. 39–55.
Price, J.T., Gransden, J.F., Khan, M.A., Ryan, B.D., 1992. Effects
of selected minerals on high temperature properties of coke.
Proc. 2nd Int. Cokemaking Cong., The Institute of Materials,
London, vol. 1, pp. 287–292.
Ragan, S., Marsh, H., 1980. A critique of industrial methods of
measurement of strength of metallurgical coke. J. Phys. D:
Appl. Phys. 13, 983–993.
M.A. Dıez et al. / International Journal of Coal Geology 50 (2002) 389–412 411
Rooney, K.A., Gregory, O.R., Nightingale, R.J., Price, K., 1987.
Developments in coke quality and the improved performance of
a 300 cubic meter blast furnace. Preprints 1st Int. Cokemaking
Cong., Essen, vol. 1, C3, 17 pp.
Rudyka, V., 2000. Main trends of development of cokemaking
facilities in Ukraine. The view and assessment of Giprokoks.
Cokemak. Int. 12 (2), 66–67.
Sakawa, M., Sakurai, Y., Hara, Y., 1982. Influence of coal charac-
teristics on CO2 gasification. Fuel 61, 717–720.
Sasaki, M., Komaki, I., Matsuura, M., Saito, K., Fukada, K., 1998.
A new carbonization process with high temperature preheating.
Proc. 57th Ironmaking Conf., ISS-AIME, pp. 803–809.
Schapiro, N., Gray, R.J., 1960. Petrographic classification applica-
ble to coals of all ranks. Proc. Illinois Min. Inst., pp. 83–90.
Schapiro, N., Gray, R.J., 1964. The use of coal petrography in
cokemaking. J. Inst. Fuel 43, 234–242.
Schapiro, N., Gray, R.J., Eusner, G.R., 1961. Recent developments
in coal petrography. Blast Furnace, Coke Oven and Raw Mate-
rials Committee, Proceedings, ISS-AIME, vol. 20, pp. 89–112.
Sciazko, M., 2000. Future of coke production in Poland. Cokemak.
Int. 12 (2), 63–64.
Sirgado, M., Verduras, J.L., 1978. Coking of complex coal mix-
tures, pre-estimating of ironmaking coke quality and develop-
ment of an economical optimization pattern for coking mixtures.
Proc. Int. Iron and Steel Cong., Chicago, 404–420.
Spackman, W., 2000. History of applied coal petrology in the
United States: II. A personalized history of the origin and devel-
opment of applied coal petrology at the Pennsylvania State Uni-
versity. Int. J. Coal Geol. 42, 103–114.
Stach, E., Mackowski, M.Th., Teichmuller, M., Taylor, G.H., Chan-
dra, D., Teichmuller, R., 1982. Stach’s Textbook of Coal Petrol-
ogy, 3rd ed. Gebruder Borntraeger, Berlin.
Steyn, J.G.D., Smith, C.H., 1977. Coal petrography in the evalua-
tion of South African coals. Coal, Gold and Base Minerals of
Southern Africa, pp. 107–117.
Stopes, M.C., 1919. On the four visible ingredients of banded bi-
tuminous coals. Proc. R. Soc. B 90, 470–487.
Stopes, M.C., 1935. On the petrology of banded bituminous coals.
Fuel 14, 4–13.
Strauss, A.D., 1999. Evaluation of metallurgical coal blends in the
Calderon coking reactor. Cokemaking Technology. Technical
Exchange Session. Int. Iron and Steel Institute (IISI), Committee
on Technology, Brussels, pp. 9–15.
Suarez-Ruiz, I., 2000. Coal petrology and reflectance microscopy.
In: Marsh, H., Rodrıguez-Reinoso, F. (Eds.), Sciences of Carbon
Materials. Secretariado de Publicaciones, Chap. 16. The Univer-
sity of Alicante, Spain, pp. 533–569.
Taketomi, H., Nishioka, K., NaKashima, Y., Suyama, S., Matsuura,
M., 2000. Research on coal pre-treatment process of Scope 21.
Proc. 4th European Coke and Ironmaking Cong., ATS-RM,
Paris, vol. 2, pp. 640–645.
Taylor, G.H., 1957. The behaviour of petrological components of
coal on carbonization. Fuel 36, 221–235.
Taylor, G.H., Mackowsky, M.Th., Alpern, B., 1967. The behaviour
of inertinite during carbonisation. Fuel 46, 431–440.
Terjung, J., 2000. World coal and coke market presence and future.
Proc. 4th European Coke and Ironmaking Cong., ATS-RM,
Paris, vol. 2, pp. 20–29.
Terjung, J., Hermann, W., 2000. Present tendencies on the world
coke market. Cokemak. Int. 12 (1), 32–37.
The British Carbonization Resarch Association (BCRA), 1980. The
evaluation of the Nippon Steel Corporation reactivity and post-
reaction strength test for coke. Carbonization Research Report
91, Chesterfield, UK, 50 pp.
Thompson, R.R., 2000. History of applied coal petrology in the
United States: III. Contributions to applied coal and coke pet-
rology at the Bethlehem Steel Corporation. Int. J. Coal Geol. 42,
Thompson, R.R., Benedict, L.G., 1976. Coal composition and its
influence on cokemaking. Iron Steelmak. 3 (2), 21–31.
Trickett, A., 1999. The outlook for coke supply and demand.
Cokemak. Int. 11 (1), 28–31.
Tucker, J., Everitt, G., 1992. Coking pressure—its causes, measure-
ment and control. Proc. 2nd Int. Cokemaking Cong., vol. 2. The
Institute of Materials, London, pp. 40–61.
United Nations Economic Commission for Europe (UNECE), 1965.
Method of measuring reactivity of metallurgical coke. ST-ECE-
COAL-12, United Nations New York, 17 pp.
Valia, H.S., 1987. Predicting coke strength after reaction with CO2
from coal analysis. Proc. 46th Ironmaking Conf., ISS-AIME,
Valia, H.S., 1989. Prediction of coke strength after reaction with
CO2 from coal analyses at Inland Steel Company. Iron Steel-
mak., 77–87 (also in: Coke Reactivity and its Effect on Blast
Furnace Operation, ISS-AIME, 1990, pp. 109–119).
Vander, T., Alvarez, R., Ferraro, M., Fohl, J., Hofherr, K., Huart,
J.M., Mattila, E., Propson, R., Willmers, R.R., van der Velden,
B., 1996. Coke quality improvement. Possibilities and limita-
tions. Proc. 3rd European Ironmaking Cong., CRM-VDEh, Gent,
Belgium, pp. 28–37 (also in: The Coke Oven Managers’
Association (COMA) Year-Book, Rotherham, UK, 1997,
Vogt, D., 2000. Coke strength after reaction. Signification regarding
with various operation and various cokes. Proc. 59th Ironmak-
ing Conf., ISS-AIME, pp. 47–54.
Walker, D.N., 1999. Sun Coke heat recovery coke technology at
Indiana Harbor. Cokemaking technology. Technical Exchange
Session. Int. Iron and Steel Institute (IISI), Committee on Tech-
nology, Brussels, pp. 1–8.
Wessiepe, K., Karsten, E., 2000. Recent developments in the world
coke industry. Coke demand/coke production. Cokemak. Int. 12
Westbrook, R.W., Schuett, K.J., 2000. Two years of heat recovery
coke production at Sun coke company’s Indiana Harbor facility.
Proc. 4th European Coke and Ironmaking Cong., ATS-RM,
Paris, vol. 2, pp. 654–658.
M.A. Dıez et al. / International Journal of Coal Geology 50 (2002) 389–412412